Four Metalloporphyrinic Frameworks as Heterogeneous Catalysts for Selective Oxidation and Aldol Reaction
Chao Zou; Tianfu Zhang; Ming-Hua Xie; Lijun Yan; Guo-Qiang Kong; Xiu-Li Yang; An Ma; Chuan-De Wu; Inorganic Chemistry 52 (2013) 3620–3626; doi:10.1021/ic3019502

data_4334265
_publ_section_title
;
 Four Metalloporphyrinic Frameworks as Heterogeneous Catalysts for
 Selective Oxidation and Aldol Reaction
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              3620
_journal_page_last               3626
_journal_paper_doi               10.1021/ic3019502
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'C67 H73 Mn N10 O19 Zn2'
_chemical_formula_weight         1508.03
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   16.6701(12)
_cell_length_b                   16.6701(12)
_cell_length_c                   15.481(2)
_cell_measurement_reflns_used    9022
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      22.94
_cell_measurement_theta_min      1.73
_cell_volume                     4302.0(7)
_computing_cell_refinement       'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_data_collection       'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_data_reduction        'CrysAlisPro (Oxford Diffraction Ltd., 2010)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.3592
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Xcalibur, Atlas, Gemini ultra'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0751
_diffrn_reflns_av_sigmaI/netI    0.0310
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            9022
_diffrn_reflns_theta_full        22.94
_diffrn_reflns_theta_max         22.94
_diffrn_reflns_theta_min         1.73
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    0.761
_exptl_absorpt_correction_T_max  0.922
_exptl_absorpt_correction_T_min  0.846
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   CrysAlisPro
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    1.164
_exptl_crystal_description       block
_exptl_crystal_F_000             1564
_exptl_crystal_size_max          0.31
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.11
_platon_squeeze_details
;
There are about one (CH~3~)~2~NH~2~, five DMF and two H~2~O disordered 
lattice molecules were removed from the formular unit 
by the SQUEEZE process.
;
_refine_diff_density_max         0.590
_refine_diff_density_min         -0.276
_refine_diff_density_rms         0.047
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     65
_refine_ls_number_reflns         893
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0443
_refine_ls_R_factor_gt           0.0358
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0487P)^2^+1.8119P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0870
_refine_ls_wR_factor_ref         0.0897
_reflns_number_gt                759
_reflns_number_total             893
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic3019502_si_002_1.cif
_cod_data_source_block           Zn-MnTCPP
_cod_database_code               4334265